Application Process for European Furniture
|Application Process for European Furniture|
|Substrate: Veneered board, solid wood||Temperature: 25℃||Humidity: 75%|
|Serial No.||Procedure||Drying time||Application method||Main points for mixing and operation|
|1||Distressing||－||Manual||Tapping, filing edge, slot broaching, wormhole|
|2||Blank sanding||－||Machine polish/manual polish||240--320#sandpaper is used to remove stains and sand marks and polish to make it smooth|
|3||Material adjustment||5 minutes||Spray||Red or green water, adjust specific material color difference|
|4||Ground color||－||Spray||Coloring agent, spray uniformly according to the color chart|
|5||PU sealer||4-8 hours||Spray||PU sealer (9-10 seconds), spray uniformly|
|6||Polish||－||Manual polish||320#-400# sand paper is used to polish slightly to make the surface smooth. Polish through is strictly prohibited.|
|7||Glaze||4-8 hours||Wipe||Wipe with glaze according to the color chart uniformly|
|8||Primer||1-2 hours||Spray||Transparent primer (11-13 seconds) and spray uniformly two cross shapes.|
|9||Polish||－||Manual polish||320#-400# sand paper is used to polish slightly to make the surface smooth. Polish through is strictly prohibited.|
|10||Crack paint||1-2 hours||Spray||Transparent crack paint (11-13 seconds), spray slightly in edge, corner and carve patterns|
|11||Gold/silver tracing||1-2 hours||Manual||Trace carving, edge and lines with gold/silver powder paint|
|12||Dry brushing||1-2 hours||Brushing||Brush Glaze on gold powder paint, crack paint and edge.|
|13||Primer||8-12 hours||Spray||Transparent primer (13-15 seconds) and spray uniformly one cross shape.|
|14||Polish||－||Manual polish||320#-400# sand paper is used to polish slightly to make the surface smooth. Polish through is strictly prohibited.|
|15||Spot spray||5 minutes||Spray||Coloring agent, spot spray according to the color chart|
|16||Repairing top coat||5 minutes||Spray||Repairing top coat (9-10 seconds), repair uniformly according to the color chart|
|17||Matte varnish||24-48 hours||Spray||Matte varnish (11-14 seconds) and spray uniformly two cross shapes.|
1、This process is suitable for products exporting to Europe, suite furniture, hotel furniture and other European style furniture.
2、According to the product requirements, the third production procedure can be omitted while making medium grade furniture and medium grade hotel furniture. In case of PU series paint, the tenth procedure in this process can be omitted.
3、Special attention shall be paid to the water content of the substrate. The substrate shall be dried to the equivalent water content level of local wood.
4、In summer, if the weather is of high temperature and high humidity, corresponding measures shall be taken to avoid whitening, blistering, pinholes and other faults in such environment; In winter, the temperature is low and corresponding measures shall be taken to avoid slow drying, sagging, ribbing, mixing with sand, dents, after-tack and other faults.
5、Special attention shall be paid to the viscosity of the sprayed paint, which is the fundamental condition to ensure paint film quality. For the paint spray viscosity listed in this process table (for example, matte top coat 11-14 seconds), it shall depend on the temperature while spraying to determine if it is proper to spray 11 seconds or 14 seconds. During summer application, the largest spray viscosity is 12 seconds, while in winter application, the smallest spray viscosity is 12 seconds.
6、The viscosity of sprayed paint in this process subject to the measurement of IWATA No.2 cup.
7、If there is requirement for low odor, odorless products can be used.
8、To ensure the paint quality in this process, all the paint used in this process must be the matching paint.